Sep 11, 2012 - 1Department of Applied Physics, Birla Institute of Technology, ... 9.2.3 Degenerate Bright Screening PV Bistable Solitons . ..... First two terms do not involve spatial integration, therefore, they ..... strength of Ep and the input intensity of soliton forming optical beam. ..... Depending on the symmetry class of.
SOME ASPECTS OF OPTICAL SPATIAL SOLITONS IN PHOTOREFRACTIVE CRYSTALS S. Konar1 and Anjan Biswas2 1 Department of Applied Physics, Birla Institute of Technology, Mesra, Ranchi-835215, Jharkhand, India
arXiv:1209.2211v1 [physics.optics] 11 Sep 2012
Department of Mathematical Sciences, Delaware State University, Dover, DE 19901-2277, USA 11 September, 2012
Abstract We have reviewed recent developments of some aspects of optical spatial solitons in photorefractive media. Underlying principles governing the dynamics of photorefractive nonlinearity have been discussed using band transport model. Nonlinear dynamical equations for propagating solitons have been derived considering single as well as two-photon photorefractive processes. Fundamental properties of three types of solitons, particularly, screening, photovoltaic and screening photovoltaic solitons have been considered. For each type of solitons, three different configurations i.e., bright, dark and gray varieties have been considered. Mechanisms of formation of these solitons due to single as well as two-photon photorefractive processes have been considered and their self bending discussed. Vector solitons, particularly, incoherently coupled solitons due to single photon and two-photon photorefractive phenomena have been highlighted. Existence of some missing solitons have been also pointed out.
Contents 1 Introduction
2 Photorefractive Effect
3 Origin of Photorefractive Nonlinearity
4 Band Transport Model
5 Space Charge Field
6 Photorefractive Nonlinearity
7 Classification of Photorefractive Solitons 7.1 Solitons Due to Single Photon Photorefractive Phenomenon . . . 7.2 Nonlinear Equation for Solitons . . . . . . . . . . . . . . . . . . . . 7.3 Bright Screening Spatial Solitons . . . . . . . . . . . . . . . . . . . 7.3.1 Bistable Screening Solitons . . . . . . . . . . . . . . . . . . 7.4 Dark Screening Solitons . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Gray Screening Solitons . . . . . . . . . . . . . . . . . . . . . . . . 7.6 Self Deﬂection of Bright Screening Solitons . . . . . . . . . . . . . 7.7 Photovoltaic and Screening Photovoltaic Solitons . . . . . . . . . 7.8 Self Deﬂection of Photovoltaic and Screening Photovoltaic Solitons
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
7 7 8 9 10 10 11 12 13 14
8 Two-Photon Photorefractive Phenomenon 8.1 Two-Photon Photorefractive Nonlinearity . 8.2 Nonlinear Evolution Equation . . . . . . . 8.3 Screening Solitons . . . . . . . . . . . . . . 8.4 Photovoltaic Solitons . . . . . . . . . . . . 8.5 Screening Photovoltaic Solitons . . . . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
15 15 17 17 19 20
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
. . . . .
Vector Solitons 9.1 Two Component Incoherently Coupled Vector Solitons . . . . . . . . . . . . . . . . . . . . 9.1.1 Coupled Solitary Wave Equations Due to Single Photon Phenomenon . . . . . . . 9.2 Incoherently Coupled Screening Vector Solitons . . . . . . . . . . . . . . . . . . . . . . . 9.2.1 Missing Bright Screening PV Solitons . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.2 Stationary Composite Solitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.3 Degenerate Bright Screening PV Bistable Solitons . . . . . . . . . . . . . . . . . . 9.2.4 Numerical Simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Incoherently Coupled Solitons Due to Two-Photon Photorefractive Phenomenon . . . . . 9.3.1 Incoherently Coupled Two-Photon Photovoltaic solitons Under Open Circuit Condition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 126.96.36.199 Bright-dark solitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 188.8.131.52 Bright-bright solitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 184.108.40.206 Dark-dark solitons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
10 Conclusion List of Figures50
21 22 22 23 24 26 27 27 28 29 29 30 31 32
Introduction The advent of nonlinear optics has paved the way to a number of fundamental discoveries. Exotic
one, among many of these, is the discovery of optical solitons [1–16]. These are optical pulses or beams which are able to propagate without broadening and distortion. Optical solitons are envelope solitons, and the term soliton was ﬁrst coined by Zabusky and Kruskal in 1965 to reﬂect the particle like nature of these waves that remain intact even after mutual collision . Optical solitons are extensively studied topic not solely due to their mathematical and physical elegance but as well as due to the possibility of real life applications. They have been contemplated as the building blocks of soliton based optical communication systems, signal processing, all optical switching, all optical devices etc. In optics, three diﬀerent types of solitons are known till date, these are, temporal [2, 3], spatial [5, 6] and spatio-temporal solitons [7, 8]. Temporal solitons are short optical pulses which maintain their temporal shape while propagating over long distance. The way a temporal optical soliton is established is that a nonlinear pulse sets out in dispersive medium and develops a chirp. Then the dispersion produces a chirp of opposite sign. A temporal soliton pulse results due to the balancing of these opposite chirps across the width of the pulse, which arise from the material dispersion and nonlinearity.These opposite chirps balance each other when dispersion is completely canceled by the nonlinearity of the medium. Temporal solitons are routinely generated in optical ﬁbers  and they are backbone of soliton based optical communication systems, soliton lasers etc. In contrast, optical spatial solitons are beams of electromagnetic energy that rely upon balancing diﬀraction and nonlinearity to retain their shape. While propagating in the nonlinear medium, the optical beam modiﬁes the refractive index of the medium in such a way that the spreading due to diﬀraction is eliminated. Thus, optical beam induces a nonlinear waveguide and at the same time guided in the waveguide it has induced. This means soliton is a guided mode of the nonlinear waveguide induced by it. Though temporal solitons can be easily generated in optical ﬁbers, generation of spatial optical solitons is a much more diﬃcult task. For example, in silica glass, the nonlinearity is proportional to light intensity and the value of the proportionality constant n2 is of the order of 10−16 cm2 /W only. Therefore, in order to compensate for the beam spreading due to diﬀraction, which is a large eﬀect, required optical nonlinearity is very large, and, consequently optical power density is also large . Another impediment in detecting spatial solitons, in bulk Kerr nonlinear media, is the catastrophic collapse of the optical beam, which is inevitable with Kerr nonlinearity. Discovery of non Kerr nonlinearities, whose mechanism is diﬀerent from Kerr nonlinearity, has lead to the revelation of stable three dimensional soliton formations without catastrophic collapse. These nonlinearities are photorefractive nonlinearity [10, 18], quadratic nonlinearity [19–22] and resonant electronic nonlinearity in atoms or molecules [23–27]. With the identiﬁcation of photorefractive nonlinearity, which possesses strong nonlinear optical response, it is possible to create optical solitons at very low light intensity. Spatial photorefractive optical solitons possess some unique properties which make them attractive in several applications, such as, all optical switching and routing, interconnects, parallel computing, optical storage etc [15, 16, 28, 35]. They are also promising for experimental veriﬁcation of theoretical models, since, they can be created at very low power. In the present article, we conﬁne our discussion on the properties of photorefractive spatial solitons.
The photorefractive(PR) eﬀect is the change in refractive index of certain electro-optic materials owing to optically induced redistribution of charge carriers. Light induced refractive index change occurs owing to the creation of space charge ﬁeld, which is formed due to nonuniform light intensity. Originally the photorefractive eﬀect was considered to be undesirable, since this leads to scattering and distortion of collimated optical beams . Soon it was realized that these materials have potential applications in holography , optical phase conjugation , optical signal processing and optical storage [34, 35]. Photorefractive materials are classiﬁed in three diﬀerent categories. Most commonly used photorefractive materials are inorganics, such as, LiN bO3 , BaT iO3 , Srx Br1−x N b2 O6 , KN bO3 , Bi12 SiO20 , Bi12 T iO20 (BT O) etc. Semiconductors have large carrier mobility that produces fast dielectric response time, which is important for fast image processing. Therefore, photorefractive semiconductors, such as, GaAs, InP, CdTe etc., complement the photorefractive ferroelectrics with the potential of fast holographic processing of optical information. Polymers also show strong photorefractive eﬀect [37–40]. They are easy to produce and PR eﬀect in polymers appear only if a high voltage is applied. Strong photorefractive pattern can be erased easily in polymers by decreasing the applied voltage. Polymers show good temperature stability, and for a given applied voltage, they usually show stronger refractive index change in comparison to inorganic crystals with equal doping densities.
Origin of Photorefractive Nonlinearity
In a photorefractive material, the spatial distribution of intensity of the optical ﬁeld gives rise to an inhomogeneous excitation of charge carriers. These charge carriers migrate due to drift and or diﬀusion and produce a space charge ﬁeld, whose associated electric ﬁeld modiﬁes the refractive index of the crystal via Pockel’s eﬀect [32, 34, 35]. For a noncentrosymmetric photorefractive crystal, the refractive index change due to the linear electro-optic eﬀect is given by [32, 34] 1 ∆n = − n3 ref f Esc , 2
where n is the average refractive index, ref f is the eﬀective linear electro-optic coeﬃcient which depends on the orientation of the crystal and polarization of light, and Esc is the space charge ﬁeld. A unique feature of photorefractive materials is their ability to exhibit both self focusing and defocusing nonlinearity in the same crystal. This is achieved by changing the polarity of the biased ﬁeld, which in turn changes the polarity of the space charge ﬁeld Esc . Hence, the same crystal can be used to generate either bright ( require self focusing nonlinearity) or dark and gray solitons ( require defocusing nonlinearity). Photorefractive nonlinearity is also wavelength sensitive, thus, it is possible to generate solitons at one wavelength and then use the soliton supported channel to guide another beam at diﬀerent wavelength.
Band Transport Model
The most widely accepted theoretical formulation of photorefractive phenomenon is described by KukhtarevVinetskii band transport model . A schematic diagram of this model is shown in ﬁgure (1), where a PR crystal is being illuminated by an optical beam with nonuniform intensity. Insert Figure (1) here The photorefractive medium, at the ground level, has completely full valance band and an empty conduction band. The material has both donor and acceptor centers, uniformly distributed, whose energy 4
states lies somewhere in the middle of the band gap. The acceptor electron states are at much lower energy in comparison to that of the donor electron states. The presence of a nonuniform light beam excites unionized donor impurities, creates charge carriers which move to the conduction band where they are free to move to diﬀuse or to drift under the combined inﬂuence of self generated and external electric ﬁeld and are ﬁnally trapped by the acceptors. During this process, some of the electrons are captured by ionized donors and thus are neutralized. In the steady state, the process leads to the charge separation, which tends to be positive in the illuminated region and vanish in the dark region. We assume that the donor impurity density is ND and acceptor impurity density NA . If the + ionized donor density is ND , then the rate of electron generation due to light and thermal processess is + (si I + βT )(ND − ND ), where si is the cross section of photoexcitation, I is the intensity of light which is written in terms of Poynting ﬂux I = 2ηn0 |Φ|2 , Φ is the electric ﬁeld of light, ǫ0 is the free space
permittivity, and βT is the rate of thermal generation. If N is the electron density and γR the electron trap recombination coeﬃcient, then, the rate of recombination of ionized donars with free electrons is + γR N N D . Thus, the rate equation describing the donar ionization is given by + ∂ND + + = (si I + βT )(ND − ND ) − γR N N D . ∂t
The electron concentration is aﬀected by recombination with ionized donors and due to migration of electrons, resulting in an electron current with current density J, hence, electron continuity equation turns out to be + →− → ∂ND 1− ∂N − = ∇. J , ∂t ∂t e
and − → → − → − + J = eN µ E + kB T µ ∇N + kp si ND − ND I~c,
→ − where the current density J is the sum of the contributions from the drift, diﬀusion and photovoltaic eﬀect; e is the electronic charge, µ is the electron mobility, kB is the Boltzmann constant, T is electron temperature, kp is the photovoltaic constant and ~c is the unit vector in the direction of c-axis of the PR crystal. E is the total electric ﬁeld including the one externally applied and that associated with the generated space charge. The redistribution of electrical charges and the creation of space charge ﬁeld obey the Poisson’s equation, therefore, → − − → ∇ · ǫ E = ρ, (5) and the charge density ρ is given by → + ρ (− r ) = e ND − NA − N .
Equations (2) -(6) can be solved to ﬁnd out the space charge ﬁeld Esc and subsequently the optical nonlinearity in the photorefractive media.
Space Charge Field
To estimate the nonlinear index change in photorefractive media due to the presence of nonuniform optical ﬁeld, we need to calculate the screening electric ﬁeld Esc . The response of a photorefractive material to the applied optical ﬁeld is anisotropic and it is nonlocal function of light intensity. Anisotropy does not 5
allow radially symmetric photorefractive solitons [42, 43]. To formulate a simple problem, and since, most of the experimental investigations on photorefractive solitons are one dimensional waves, it is appropriate to ﬁnd material response in one dimension ( say x only). Steady state photorefractive solitons may be obtained under homogeneous background illumination, which enhances dark conductivity of the crystal. In the steady state, induced space charge ﬁeld Esc can be obtained from the set of rate, continuity, current equations and Gauss law. In the steady state, and in one dimension, these equations reduce to [44–46]: + + si (I + Id )(ND − ND ) − γR N N D = 0,
e ∂Esc (N + − NA − N ), = ∂x ǫ0 ǫr D
J = eN µEsc + kB T µ
∂N + + kp si ND − ND I, ∂x
∂J = 0, ∂x where ǫr is the relative static permittivity; Id (=
) is the so called dark irradiance that phenomeno-
logically accounts for the rate of thermally generated electrons. This is also the homogeneous intensity that controls the conductivity of the crystal. In most cases, the optical intensity I is such that for electron + dominated photo-refraction, N ≪ ND , N ≪ NA and NA ≪ ND . Under this usually valid situation, the space charge ﬁeld Esc is related to the optical intensity I through
Esc = E0
1 ∂I I∞ − I kB T I∞ + ID + Ep − , I + ID I + ID e I + ID ∂x
(11) k γ N
R A is the photovoltaic where Eo is the external bias ﬁeld to the photorefractive crystal, Ep = p eµ ﬁeld. In addition, we have assumed that the power density of the optical ﬁeld attains asymptotically a
constant value at x → ±∞ i.e., I(x → ±∞, z) = I∞ . Moreover, in the region of constant illumination, equations(7)-(10) require that the space charge ﬁeld Esc is independent of x i.e., Esc (x → ±∞, z) = Eo .
The space charge induced change △n in the refractive index n is obtained as
I∞ + ID 1 ∂I 1 3 I∞ − I kB T . |△n| = n ref f E0 + Ep − 2 I + ID I + ID e I + ID ∂x
It is evident from above expression that the change in refractive index is intensity dependent, i.e., under the action of nonuniform illumination the photorefractive crystal has become an optical nonlinear medium. The ﬁrst term in the above equation is generally known as the screening term. In nonphotovoltaic photorefractive material, this is the main term which is responsible for soliton formation. The space charge redistribution in a photorefractive crystal is caused mainly by the drift of photoexcited charges under a biasing electric ﬁeld. This mechanism leads directly to a local change of refractive index and is responsible for self-focusing of optical beams. The second term is due to photovoltaic eﬀect, which leads to the formation of photovoltaic solitons. First two terms do not involve spatial integration, therefore, they are local nonlinear terms. Functional form of both terms are diﬀerent from Kerr nonlinearity. These terms are similar to that of saturable nonlinearity and explain why the collapse phenomenon is not observable
in photorefractive materials. Besides drift mechanism, transport of charge carriers occurs also due to diﬀusion process. This process results in the nonlocal contribution to the refractive index change. The last term is due to diﬀusion. The strength of the diﬀusion eﬀect is determined by the width of the soliton forming optical beam. In case of strong bias ﬁeld and relatively wide beams, the diﬀusion term is often neglected. However, its contribution can become signiﬁcant for very narrow spatial solitons or optical beams. When diﬀusion is signiﬁcant, it is responsible for deﬂection of photorefractive solitons [44–46].
Classification of Photorefractive Solitons Solitons Due to Single Photon Photorefractive Phenomenon
Till date, three diﬀerent types of steady state spatial solitons have been predicted in photorefractive media, which owe their existence due to single photon photorefractive phenomenon. Photorefractive screening solitons were identiﬁed ﬁrst. In the steady state, both bright and dark screening solitons (SS) are possible when an external bias voltage is appropriately applied to a non-photovoltaic photorefractive crystal [47–56]. Intuitively, the formation of bright screening photorefractive solitons can be understood as follows. When a narrow optical beam propagates through a biased photorefractive crystal, as a result of illumination, conductivity in the illuminated region increases and the resistivity decreases. Since the resistivity is not uniform across the crystal, the voltage drops primarily across the non illuminated region and voltage drop is minimum in the high intensity region. This leads to the formation of large space charge ﬁeld in the dark region and much lower ﬁeld in the illuminated region. The applied ﬁeld is thus partially screened by the space charges induced by the soliton forming optical beam. The refractive index changes which is proportional to this space charge ﬁeld. The balance of self diﬀraction of the optical beam by the focusing eﬀect of the space charge ﬁeld induced nonlinearity leads to the formation of spatial solitons. These screening solitons were ﬁrst predicted by Segev et. al. , whereas, the experimental observation of bright SS were reported by M.Shih et. al.  and those of dark SS were reported by Z. Chen et. al. . The second type PR soliton is the photovoltaic solitons [57–61], the formation of which, however, requires an unbiased PR crystal that exhibits photovoltaic eﬀect, i.e., generation of dc current in a medium illuminated by a light beam. The photovoltaic (PV) solitons owe their existence to bulk photovoltaic eﬀect, which creates the space charge ﬁeld, that, in turn modiﬁes the refractive index and gives rise to spatial solitons. These solitons were ﬁrst predicted by G. C. Valey et. al.  and observed experimentally in 1D by M.Taya et.al.  and in 2D by Z.Chen et. al. . Two dimensional bright photovoltaic spatial solitons were also observed in a Cu:KNSBN crystal by She et. al. . The observed spatial solitons were broader than those predicted by considering Esc due to signal beam alone. This was satisfactorily explained by an equivalent ﬁeld induced by the background ﬁeld. The third type of photorefractive solitons arises when an electric ﬁeld is applied to a photovoltaic photorefractive crystal [31, 60, 61, 63, 64]. These solitons, owe their existence to both photovoltaic eﬀect and spatially nonuniform screening of the applied ﬁeld, and, are also known as screening photovoltaic (SP) solitons. It has been veriﬁed that, if the bias ﬁeld is much stronger than the photovoltaic ﬁeld, then, the screening photovoltaic solitons are just like screening solitons. On the other hand, if the applied ﬁeld is absent, then SP solitons degenerate into photovoltaic solitons in the closed circuit condition. The ﬁrst observation of bright photovoltaic screening solitons in LiN bO3 was reported by E. Fazio et. al. .
Nonlinear Equation for Solitons
In order to develop a semi analytical theory, one dimensional reduction is introduced in the subsequent discussion. The optical beam is such that no y dynamics is involved and it is permitted to diﬀract only → − along x direction. Electric ﬁeld E of the optical wave and the bias ﬁeld E0 are directed along the x axis which is also the direction of the crystalline c-axis. Under this special arrangement, the perturbed extraordinary refractive index n ˆ e is given by [45, 46, 60] (ˆ ne )2 = n2e − n4e ref f Esc ,
where ne is the unperturbed extraordinary index of refraction. This arrangement allows us to describe → − the optical beam propagation using Helmholtz’s equation for the electric ﬁeld E , which is as follows: → − → − ∇2 E + (k0 n ˆ e )2 E = 0,
where k0 = 2π λ0 and λ0 is the free space wavelength of the optical ﬁeld. Moreover, if we assume − → → − E = x Φ(x, z)exp[i(kz − ωt)], where k = k0 ne and employ slowly varying envelope approximation for the amplitude Φ, then, the Helmholtz’s equation can be reduced to the following parabolic equation: i
∂Φ 1 ∂2Φ 1 − k0 n3e ref f Esc Φ = 0. + ∂z 2k ∂x2 2
The space charge ﬁeld that has been evaluated earlier in section(5) can be employed in the above equation to obtain following nonlinear Schr¨odinger equation: i
where ξ =
A (ρ − |A|2 )A A ∂|A|2 ∂A 1 ∂ 2 A − β(1 + ρ) −α +δ + = 0, 2 2 2 2 ∂ξ 2 ∂s 1 + |A| 1 + |A| 1 + |A| ∂s
z , k0 ne x20
x x0 ,
I∞ Id ,
β = (k0 x0 )2 (n4e ref f /2)E0 , α = (k0 x0 )2 (n4e ref f /2)Ep , A =
ne 2η0 Id Φ
and δ = (k02 x0 ref f n4e kB T )/(2e). Equation (16) gives rise to varieties of solitons depending on speciﬁc experimental situations. Important parameters which classify these solitons and govern their dynamics are α and β. The parameter δ, which is associated with the diﬀusion term, is not directly responsible for soliton formation. The diﬀusion processes is primarily responsible for bending of trajectories of propagating solitons, hence, large value of δ inﬂuences the trajectory of bending. The dimensionless parameter β can be positive or negative depending on the sign of E0 i.e., the polarity of external applied
ﬁeld. In non-photovoltaic photorefractive media α = 0, therefore, if we neglect the diﬀusion term, which is small indeed, and introduce only ﬁrst order correction, then β is the parameter which governs the soliton formation. The relevant dynamical equation in non-photovoltaic photorefractive media turns out to be A ∂A 1 ∂ 2 A − β(1 + ρ) = 0. (17) + i ∂ξ 2 ∂s2 1 + |A|2 This is the modiﬁed nonlinear Schr¨odinger equation(MNLSE) with saturable nonlinearity which is not integrable. The term 1/(1 + |A|2 ) represents local saturable nonlinear change of refractive index of the crystal induced by the optical beam. The saturating nature of the nonlinearity will be more clearly evident if we make the transformation A = u exp[−iβ(1 + ρ)ξ], in which case above equation reduces to i
∂u 1 ∂ 2 u |u|2 + β(1 + ρ) u = 0. + 2 ∂ξ 2 ∂s 1 + |u|2
It will be shown subsequently that a positive β is essential for creation of bright spatial solitons, whereas, a negative β leads to the formation of dark or gray solitons. Thus, by changing the polarity of the external applied ﬁeld, it is possible to create bright as well as dark solitons in the same photorefractive media. Equation(17) has been extensively investigated for bright, dark as well as gray solitons [46, 60, 61]. In the next section, we consider bright screening spatial solitons using a method outlined by Christodoulides and Carvalho  and subsequently employed in a large number of investigations [108– 111, 137, 145, 146].
Bright Screening Spatial Solitons
We ﬁst consider bright screening solitons for which the soliton forming beam should vanish at inﬁnity (s → ±∞), and thus, I∞ = ρ = 0. Therefore, bright type solitary waves should satisfy i
∂A 1 ∂ 2 A A −β = 0. + 2 ∂ξ 2 ∂s 1 + |A|2
We can obtain stationary bright solitary wave solutions by expressing the beam envelope as A(s, ξ) = 1 2
p y(s) exp(iνξ), where ν is the nonlinear shift in propagation constant and y(s) is a normalized real function which is bounded as, 0 ≤ y(s) ≤ 1. The quantity p represents the ratio of the peak intensity
(Imax ) to the dark irradiance Id , where Imax = I(s = 0). Furthermore, for bright solitons, we require y(0) = 1, y(0) ˙ = 0 and y(s → ±∞) = 0 . Substitution of the ansatz for A(s, ξ) into equation(19) yields y d2 y − 2νy − 2β = 0. 2 ds 1 + py 2
Integration of above equation once and use of boundary condition yields ν = −(β/p) ln(1 + p),
= (2β/p)[ln(1 + py 2 ) − y 2 ln(1 + p)].
By virtue of integration of above equation, we immediately obtain 1 s=± (2β)1/2
p1/2 db y. [ln(1 + pb y 2 ) − yb2 ln(1 + p)]1/2
The nature of above integrand is such that it does not provide any closed form solution. Nevertheless, the normalized bright proﬁle y(s) can be easily obtained by the use of simple numerical procedure. It can be easily shown that the quantity in the square bracket in equation(23) is always positive for all values of y 2 between 0 ≤ y(s) ≤ 1. Therefore, the bright screening photorefractive solitons can exist in a medium only when β > 0 i.e., E0 is positive. For a given value of β, the functional form of y can be obtained for diﬀerent p which determines soliton proﬁle. For a given physical system, the spatial beam width of these solitons depends on two parameters E0 and p. For illustration, we take SBN crystal with following parameters ne = 2.35, r33 = 224 × 10−12 m/V. Operating wavelength λ0 = 0.5µm, x0 = 20µm and E0 = 2 × 105 V/m. With these parameters, value of β ≃ 43. Figure (2) depicts typical normalized intensity proﬁles of bright solitons.
Insert Figure (2) here 7.3.1
Bistable Screening Solitons
Equation(19) possesses several conserved quantities, one such quantity is P =
|A|2 ds, which can be
identiﬁed as the total power of the soliton forming optical beam. Numerically evaluated soliton proﬁle |A|2 = p|y(s)|2 can be employed to calculate P . Solitons obtained from equation(23) are stable since they obey Vakhitiov and Kolokolov  stability criteria i.e., dP/dν > 0. These soliton proﬁles can be also employed to ﬁnd out spatial width τF W HM ( full width at half maximum) of solitons. Figure (3) demonstrates the variation of spatial width τF W HM with p. This ﬁgure signiﬁes the existence of twostate solitons, also known as bistable solitons, i.e., two solitons possessing same spatial width but diﬀerent power. Similar bistable solitons were earlier predicted in doped ﬁbers [66, 67]. However, these bistable solitons are diﬀerent from those which were predicted by Kaplan and others , where two solitons with same power possessing two diﬀerent nonlinear propagation constant. Insert Figure (3) here Another point worth mentioning is that, the τF W HM vs p curve in ﬁgure(3) possesses local minimum, hence, it is evident that these solitons can exist only if their spatial width is above certain minimum value. This minimum value increases with the decrease in the value of β. For illustration, the shapes of a typical pair of bistable solitons with same τF W HM but diﬀerent peak power have been depicted in ﬁgure(4). The dynamical behavior of these bistable solitons, while propagating, can be examined by full numerical simulation of equation(19), which conﬁrms their stability. Insert Figure (4) here
Dark Screening Solitons
Equation (17) also yields dark solitary wave solutions [46, 69], which exhibit anisotropic ﬁeld proﬁles with respect to s. These solitons are embedded in a constant intensity background, therefore, I∞ is ﬁnite, hence, ρ is also ﬁnite. To obtain stationary solutions, we assume A(s, ξ) = ρ1/2 y(s)exp(iνξ), where, like earlier case, ν is the nonlinear shift in propagation constant and y(s) is a normalized real odd function of s. The proﬁle y(s) should satisfy following properties: y(0) = 0, y(s → ±∞) = ±1, dy ds = s → ±∞. Substituting the form of A in equation(17) we obtain, y d2 y − 2νy − 2β(1 + ρ) = 0. ds2 1 + ρy 2
d2 y ds2
= 0 as
Integrating above equation once and employing boundary condition, we get ν = −β.
Following similar procedure as employed earlier, we immediately obtain 1 s=± (−2β)1/2
db y [(b y2
− 1) −
y 1/2 ln 1+ρb 1+ρ ]
The quantity within the square bracket in equation(26) is always positive for all values of y 2 ≤ 1, thus
β i.e., E0 must be negative so that r.h.s of equation(26) is not imaginary. An important point to note 10
is that, for a particular type of photorefractive material, for example SBN, if positive polarity of E0 is required for bright solitons, then one can observe dark solitons by changing polarity of E0 . Spatial width of these solitons depends on only two variables β and ρ i.e., E0 and I∞ . It has been conﬁrmed that, unlike their bright counterpart, dark screening photovoltaic solitons do not possess bistable property. For illustration, we take the same SBN crystal with other parameters unchanged, except in the present case E0 = −2 × 105 V/m. Therefore β ≈ −43. Figure (5) depicts normalized intensity proﬁles of dark solitons which are numerically identiﬁed using equation(26).
Insert Figure (5) here
Gray Screening Solitons
Besides bright and dark solitons, equation (17) also admits another interesting class of solitary waves, which are known as gray solitons . In this case too, wave power density attains a constant value at inﬁnity i.e., I∞ is ﬁnite, and hence, ρ is ﬁnite. To obtain stationary solutions, we assume A(s, ξ) = ρ1/2 y(s) exp[i(νξ +
Jdb s )], 2 y (b s)
where ν is again the nonlinear shift in propagation constant, y(s) is a normalized real even function of s and J is a real constant to be determined. The normalized real function satisﬁes the boundary ˙ = 0, y(s → ±∞) = 1 and conditions y 2 (0) = m(0 < m < 1), i.e., the intensity is ﬁnite at the origin, y(0)
all derivatives of y(s) are zero at inﬁnity. The parameter m describes grayness, i.e., the intensity I(0) at the beam center is I(0) = mI∞ . Substitution of the above ansatz for A in equation(17) yeilds d2 y y J2 − 2νy − 2β(1 + ρ) − = 0. ds2 1 + ρy 2 y3
Employing boundary conditions on y at inﬁnity we obtain J 2 = −2(ν + β).
Integrating equation(28) once and employing appropriate boundary condition, we immediately obtain m(1 + ρ) 1 + ρm −β +1−m . ln ν= (m − 1)2 ρ 1+ρ
= 2ν(y 2 − 1) +
2β (1 + ρ) ln ρ
1 + ρy 2 1+ρ
+ 2(ν + β)
1 − y2 y2
The normalized amplitude y(s) can be obtained by numerical integration of above equation. Note that dark solitons are a generalization of these gray solitons. Unlike bright or dark solitons, the phase of gray solitons is not constant across s, instead varies across s. Existence of these solitary waves are possible only when β < 1 and m < 1.
Self Deflection of Bright Screening Solitons
In the foregoing discussion we have neglected diﬀusion, however, the eﬀect of diﬀusion cannot be neglected when solitons spatial width is comparable with the diﬀusion length. The diﬀusion process introduces asymmetric contribution in the refractive index change which causes solitons to deﬂect during propagation. Results of large number of investigations addressing the deﬂection of photorefractive spatial solitons in both non-centrosymmetric and centrosymmetric photorefractive crystals are now available [70– 82]. Several authors have investigated self bending phenomenon using perturbative procedure [83, 84]. In this section, we employ a method of nonlinear optics [85, 86] which is diﬀerent from perturbative approach. To begin with, we take ﬁnite δ and use the following equation to study the self bending of screening bright spatial solitons i
∂(|A|2 ) A A ∂A 1 ∂ 2 A − β + + δ = 0. ∂ξ 2 ∂s2 (1 + |A|2 ) (1 + |A|2 ) ∂s
To obtain stationary solitary waves, we make use of the ansatz A(s, ξ) = A0 (s, ξ) exp[−iΩ(s, ξ)],
in equation(32). A straightforward calculation yields following equations: ∂A0 ∂A0 ∂Ω 1 ∂ 2 Ω − − A0 2 = 0, ∂ξ ∂s ∂s 2 ∂s
and ∂Ω 1 ∂ 2 A0 1 A0 − A0 + 2 ∂ξ 2 ∂s 2
δ ∂(A20 ) A0 + = 0. 1 + A20 1 + A20 ∂s
We look for a self-similar solution of (34) and (35) of the form (s − s0 (ξ))2 A00 , exp − A0 = p 2r02 f 2 (ξ) f (ξ)
Ω(s, ξ) =
(s − s0 (ξ))2 Λ1 (ξ) + (s − s0 (ξ))Λ2 (ξ) + Λ3 (ξ), 2
Λ1 = −
1 df , f (ξ) dξ
Λ2 = −
ds0 , dξ
where, r0 is a constant and f (ξ) is a parameter which together with r0 describe spatial width; in particular, r0 f (ξ) is the spatial width of the soliton and Λ3 is an arbitrary longitudinal phase function. s0 (ξ) is the location of the center of the soliton. For a nondiverging/ nonconverging soliton, f (ξ) = 1. (ξ) Moreover, we assume that initially solitons are nondiverging i.e., dfdξ = 0 at ξ = 0. Substituting for A0 2 and Ω in equation(35) and equating coeﬃcients of s and s on both sides, we obtain
1 2A200 d2 f = − β dξ 2 r04 f 3 r02 f 2
−2 A200 1+ , f
and d2 s0 (ξ) 2A2 = −δ 2 003 2 dξ r0 f
−1 A2 1 + 00 . f
Equation(39) describes the dynamics of the width of soliton as it propagates in the medium, while equation(40) governs the dynamics of the centre of the soliton. In order to ﬁnd out how a stationary soliton deviates from its initial propagation direction, we ﬁrst solve equation(39) for stationary soliton states. From equation(39), condition for stationary soliton states can be obtained as
(1 + A200 )2 r0 = 2βA200
Insert Figure (6) here Figure (6) depicts variation of solitons spatial width with the normalized peak power A200 . The curve in ﬁgure (6) is the existence curve of stationary solitons. Each point on this curve signiﬁes the existence of a stationary soliton with a given spatial width and peak power. A stationary soliton of speciﬁc power and width as described by equation(41) deviates from its initial path which can be found out by integrating equation(40). The equation of trajectory of the center of soliton is s0 (ξ) = −
Θ 2 ξ + s00 , 2
where Θ = δ r200 (1 + A200 ), s00 = s0 (ξ = 0), moreover f = 1, since we are only interested in stationary 0 solitons whose spatial shape remain invariant. Thus, the beam center follows a parabolic trajectory. The displacement of the soliton center with propagation distance has been depicted in ﬁgure (7). It is evident that the peak power of soliton inﬂuences lateral displacement of the soliton centre. The lateral 2 displacement suﬀered by the spatial soliton is given by Θ 2 ξ . Equation(42) implies that the angular displacement of the soliton center shifts linearly with the propagation distance ξ. The more explicit
expression of the angular displacement, i.e., the angle between the center of the soliton and the z axis can be easily obtained as Θξ. Insert Figure (7) here
Photovoltaic and Screening Photovoltaic Solitons
Steady state photovoltaic solitons can be created in a photovoltaic photorefractive crystal without a bias ﬁeld. These photovoltaic solitons result from the photovoltaic eﬀect [57–61] . Recently, it has been predicted theoretically that the screening-photovoltaic(SP) solitons are observable in the steady state when an external electric ﬁeld is applied to a photovoltaic photorefractive crystal [31, 78]. These SP solitons result from both the photovoltaic eﬀect and spatially nonuniform screening of the applied ﬁeld. If the bias ﬁeld is much stronger in comparison to the photovoltaic ﬁeld, then the SP solitons are just like the screening solitons. In absence of the applied ﬁeld, the SP solitons degenerate into photovoltaic solitons in the close-circuit condition. In other words, a closed-circuit photovoltaic soliton or screening soliton is a special case of the SP soliton. Thus, in the subsequent analysis, we develop theory for SP solitons and obtain solutions of photovoltaic solitons as a special case. When the diﬀusion process is ignored, the dynamics of these steady-state screening PV solitons ( bright, dark and gray) can be examined [60, 78, 88] using the following equation i
A (ρ − |A|2 )A ∂A 1 ∂ 2 A − β(1 + ρ) + − α = 0. ∂ξ 2 ∂s2 (1 + |A|2 ) (1 + |A|2 ) 13
Adopting the procedure, employed earlier, the bright soliton proﬁle of screening photovoltaic solitons  turns out to be 1/2
s(2(α + β))
p1/2 db y, [ln(1 + pb y 2 ) − yb2 ln(1 + p)]1/2
The quantity within the bracket in the right hand side is always positive for y(s) ≤ 1, thus, (α + β) must be positive for bright screening photovoltaic solitons. From equation(44), it is evident that, these bright SP solitons result both from the photovoltaic eﬀect (α 6= 0) and from spatially nonuniform screening (β 6= 0) of the applied electric ﬁeld in a biased photovoltaic-photorefractive crystal. Formation of
these solitons depends not only on the external bias ﬁeld but also on the photovoltaic ﬁeld. When we set α = 0, these solitons are just like screening solitons in a biased nonphotovoltaic photorefractive crystal . In addition, when β = 0 , we obtain expression of bright photovoltaic solitons in the close circuit realization . Thus, these SP solitons diﬀer both from screening solitons in a biased nonphotovoltaic photorefractive crystal and from photovoltaic solitons in a photovoltaic photorefractive crystal without an external bias ﬁeld. One important point to note is that the experimental conditions are diﬀerent for creation of screening, PV and SP solitons. SP solitons can be created in a biased photovoltaic-photorefractive crystal, whereas, creation of screening solitons are possible in biased nonphotovoltaic-photorefractive crystals. The PV solitons can be created in photovoltaic-photorefractive crystal without an external bias ﬁeld. We can also derive dark solitons from equation (43), the normalized dark ﬁeld proﬁle can be easily obtained as [−2(α + β)]
h (b y 2 − 1) −
db y 1+ρ ρ
i1/2 , y2 ln( 1+ρb ) 1+ρ
The condition for existence of dark solitons is (α + β) < 0. In a medium like LiN bO3 , α < 0, therefore, if |β| < |α| then the dark SP solitons can be observed irrespective of the polarity of external bias ﬁeld. However, photovoltaic constant in some photovoltaic materials, such as, BaT iO3 depends on polarization of light . This means sign of α may be positive or negative depending on polarization of light. Therefore, to observe dark SP solitons, polarization of light and external bias must be appropriate so that (α + β) < 0 . It is evident from the expression of dark solitons that, if bias ﬁeld is much stronger in comparison to the photovoltaic ﬁeld, then these SP dark solitons are just like screening dark solitons. On the other hand, if the applied external ﬁeld is absent, then these dark SP solitons degenerate into photovoltaic dark solitons in the closed circuit condition.
Self Deflection of Photovoltaic and Screening Photovoltaic Solitons
In absence of diﬀusion process, which is usually weak, photovoltaic solitons propagate along a straight line keeping their shape unchanged. However, when the spatial width of soliton is small, the diﬀusion eﬀect is signiﬁcant, which introduces an asymmetric tilt in the light-induced photorefractive waveguide, that in turn is expected to aﬀect the propagation characteristics of steady-state photorefractive solitons. Several authors [74, 78–82, 88] have examined the self bending phenomenon of PV solitons. The eﬀects of higher order space charge ﬁeld on this self bending phenomenon have been also investigated [81, 82, 88]. The deﬂection of PV bright solitons depends on the strength of photovoltaic ﬁeld. When the PV ﬁeld Ep is less than a certain characteristic value, solitons bend opposite to crystal c-axis and absolute value of 14
spatial shift due to ﬁrst order diﬀusion is always larger in comparison to that due to both ﬁrst and higher order diﬀusion . When Ep is larger than the characteristic value, direction of bending depends on the strength of Ep and the input intensity of soliton forming optical beam. Self deﬂection can be completely arrested by appropriately selecting Ep and intensity of the soliton forming optical beam. PV dark solitons experience approximately adiabatic self deﬂection in the direction of the c-axis of the crystal and the spatial shift follows an approximately parabolic trajectory. Nature of self deﬂection of PV dark solitons is diﬀerent from that of bright solitons in which self deﬂection occurs in the direction opposite to the c-axis of the crystal. Eﬀect of higher order space charge ﬁeld on self deﬂection has been also investigated , which indicates a considerable increase in the self deﬂection of dark solitons, especially under the high PV ﬁeld. Thus, the spatial shift due to both ﬁrst and higher order diﬀusion is larger in comparison to that when ﬁrst order diﬀusion is present alone. The self deﬂection of screening PV solitons depends on both the bias and PV ﬁelds . When the bias ﬁeld is positive and the PV ﬁeld is negative, the screening PV bright solitons always bend in the direction opposite to the crystal c-axis, and the absolute value of the spatial shift due to ﬁrst order diﬀusion term alone is always smaller than that due to both ﬁrst and higher order. When PV ﬁeld is positive and bias ﬁeld is negative or both are positive, then the bending direction depends both on the strength of two ﬁelds and on the intensity of the optical beam. Bending can be completely compensated for appropriate polarity of the two ﬁelds and optical beam intensity.
Two-Photon Photorefractive Phenomenon
Three types of steady state photorefractive spatial solitons, as elucidated earlier, owe their existence on the single photon photorefractive phenomenon. Recently, a new kind of photorefractive solitons has been proposed in which the soliton formation mechanism relies on two-photon photorefractive phenomenon. It is understood that the two-photon process can signiﬁcantly enhance the photorefractive phenomenon. A new model has been introduced by Castro-Camus and Magana  to investigate two-photon photorefractive phenomenon. This model includes a valance band (VB), a conduction band(CB) and an intermediate allowed level(IL). A gating beam with photon energy ¯hω1 is used to maintain a ﬁxed quantity of excited electrons from the valance band to the intermediate level, which are then excited to the conduction band by the signal beam with photon energy ¯hω2 . The signal beam induces a charge distribution that is identical to its intensity distribution, which in turn gives rise to a nonlinear change of refractive index through space charge ﬁeld. Very recently, based on Castro-Camus and Magana’s model, Hou et. al., predicted that two-photon screening solitons (TPSS) can be created in a biased nonphotovoltaic photorefractive crystal  and two-photon photovoltaic (TPPV) solitons can be also created in a PV crystal under open-circuit condition . Recently, the eﬀect of external electric ﬁeld on screening photovoltaic solitons due to two-photon photorefractive phenomenon has been also investigated [94, 95].
Two-Photon Photorefractive Nonlinearity
In order to estimate the optical nonlinearity arising out in two photon-photorefractive media, we consider an optical conﬁguration whose schematic diagram is shown in ﬁgure (8). Insert Figure (8) here
The electrical circuit consist of a crystal ( could be made of photovoltaic-photorefractive or non photovoltaic-photorefractive material), external electric ﬁeld bias voltage V and external resistance R. V0 and E0 respectively denote the potential and electric ﬁeld strength between the crystal electrodes which are separated by a distance d. Assuming the spatial extent of optical wave is much less than d, we have E0 = V0 /d; additionally V /d = Ea . Therefore, V = E0 d + JSR = Ea d,
where S is the surface area of the crystal electrodes and J is the current density. The soliton forming optical beam with intensity I2 propagates along the z direction of the crystal and is permitted to diﬀract only along the x direction. The optical beam is polarized along the x axis which is also the direction of crystal c-axis and the external bias ﬁeld is also directed along this direction. The crystal is illuminated with a gating beam of constant intensity I1 . The space charge ﬁeld Esc due to two-photon photorefractive phenomenon can be obtained from the set of rate, current, and Poisson’s equations proposed by CastroCamus et. al. . In the steady state, these equations are + + + = 0, − γR N N D ) − γ1 N i N D (s1 I1 + β1 )(ND − ND
+ + (s1 I1 + β1 )(ND − ND ) + γ2 N (Nit − Ni ) − γ1 Ni ND − (s2 I2 + β2 )Ni = 0,
(s2 I2 + β2 )Ni +
1 ∂J + − γR N N D − γ2 N (Nit − Ni ) = 0, e ∂x
∂Esc = e(Nd+ − N − Ni − NA ), ∂x
+ J = eµN Esc + κp s2 (ND − ND )I2 + eD
∂J = 0, J = constant, ∂x
∂N , ∂x
+ where ND , ND , NA and N are the donor density, ionized donor density, acceptor or trap density and density of electrons in the conduction band, respectively. Ni is the density of electrons in the
intermediate state, Nit is the density of traps in the intermediate state. κp , µ and e are respectively the photovoltaic constant, electron mobility and electronic charge; γR is the recombination factor of the conduction to valence band transition, γ1 is the recombination factor for intermediate allowed level to valence band transition, γ2 is the recombination factor of the conduction band to intermediate level transition; β1 and β2 are respectively the thermo-ionization probability constant for transitions from valence band to intermediate level and intermediate level to conduction band; s1 and s2 are photoexcitation crosses. D is the diﬀusion coeﬃcient and I2 is the intensity of the soliton forming beam. We + adopt the usual approximations ND ∼ NA and Nit − Ni 0 i.e., E0 > 0. Therefore, screening bright spatial solitons can be formed in a two-photon photorefractive medium only when external bias ﬁeld is applied in the same direction with respect to the optical c-axis. FWHM of these spatial solitons is inversely proportional to the square root of the absolute value of the external bias ﬁeld. In the low amplitude limit i.e.,when |A|2 0, i.e., Ep > 0, thus the photovoltaic ﬁeld should be in the same direction with respect to the optical c-axis of the medium. In the low amplitude limit (|A|2